Stacking Control by Molecular Symmetry of Sterically Protected Phthalocyanines

The synthesis and characterization of two phthalocyanine (Pc) structural isomers, 1 and 2, in which four 2,6-di(hexyloxy)phenyl units were attached directly to the 1,8,15,22- or 1,4,15,18-positions of the Pc rings, are described. Both Pcs 1 and 2 exhibited low melting points, i.e., 120 and 130 °C respectively, due to the reduction in intermolecular π-π interaction among the Pc rings caused by the steric hindrance of 2,6-dihexyloxybenzene units. The thermal behaviors were investigated with temperature-controlled polarizing optical microscopy, differential scanning calorimetry, powder X-ray diffraction, and absorption spectral analyses. Pc 1, having C4h molecular symmetry, organized into a lamellar structure containing lateral assemblies of Pc rings. In contrast, the other Pc 2 revealed the formation of metastable crystalline phases, including disordered stacks of Pcs due to rapid cooling from a melted liquid.


Introduction
Molecular-based functional modules have been constructed on the basis of a bottom-up approach for the designed molecular units [1][2][3]. These molecule units can be organized into hierarchical architectures through the control of the molecular shape, intermolecular noncovalent interactions, polarity of solvents, temperatures, and interactions with solid substrates [1][2][3]. The ordered orientation of the π-conjugated molecular units within the supramolecular architectures enabled highly efficient charge transportation, along with the molecular assemblies and the tuning of light absorption [4]. Phthalocyanines (Pcs) have also been used as the molecular component for the construction of supramolecular architectures [5]. Planar and disk-shaped π-conjugated Pc rings can be stacked into columnar assemblies through their strong π-π interactions. In particular, Pcs attached with flexible alkyl chains have been investigated as major thermotropic discotic liquid crystalline materials; their phase segregation between the Pc core and surrounding alkyl chains allow the creation of well-organized structures of one-dimensional columnar stacks while also keeping long-range ordering of Pc stacks within the column [6]. So far, systematic structural exploration of liquid-crystalline Pcs has been achieved by changing central metals and alkyl chains to tune the stacking modes of Pcs. However, the high viscosity and melting temperature of Pc-based liquid crystals make them poorly suited to forming large-area and uniform organized states without defects. In this study, we designed two structural isomers, 1 and 2, having different molecular symmetries (1: C 4h , 2: D 2h ) for the substitution of four 2,6-dihexyloxybenzene units at the nonperipheral positions of the Pc ring to control the stacking
Cyclic tetramerization of 3-substituted phthalonitriles usually produces a mixture of four regioisomers having different molecular symmetries (D2h, C2v, C4h, and Cs). The reaction mixture during the tetramerization of 3 at 157 °C showed a simple 1 H-NMR spectrum, suggesting the formation of a single symmetrical isomer. Several attempts for the selective formation of C4h isomers from 3-substituted phthalonitriles have been demonstrated [10][11][12]. Although the size of the methoxy groups in 3 was relatively small, as compared with the reported substituents for the successful selective formation of C4h isomers, the restriction of the dihedral angle between the two benzene rings in 3 prevented the formation of the other D2h, C2v, and Cs isomers under a high reaction temperature by keeping a good yield (48%). The methoxy groups in 5 were exchanged with hexyloxy groups by cleavage with BBr3 and subsequent ether formation. We also tried to prepare 1 from 3-(2′,6′di(hexyloxy)phenyl)phthalonitrile; however, its yield was quite low (less than 1%) under the same reaction conditions as those used for 3. The large steric hindrance of hexyloxy groups would diminish the approach of using four phthalonitriles to form the Pc ring. The resulting Pc 1 can dissolve in many solvents except for alcohol and water, and it showed sharp, simple, and assignable 1 H-NMR spectra under a 1 × 10 −2 mol/dm 3 concentration at 25 °C ( Figure 2). The wide solubilities in the solvents and the sharp 1 H-NMR peaks at a high concentration indicate good dispersion as monomeric species without the formation of intermolecular aggregates in solvents, due to the steric hindrance of 2,6dihexyloxybenzene substituents at the four α-positions of the Pc ring in 1.
Cyclic tetramerization of 3-substituted phthalonitriles usually produces a mixture of four regioisomers having different molecular symmetries (D 2h , C 2v , C 4h , and C s ). The reaction mixture during the tetramerization of 3 at 157 • C showed a simple 1 H-NMR spectrum, suggesting the formation of a single symmetrical isomer. Several attempts for the selective formation of C 4h isomers from 3-substituted phthalonitriles have been demonstrated [10][11][12]. Although the size of the methoxy groups in 3 was relatively small, as compared with the reported substituents for the successful selective formation of C 4h isomers, the restriction of the dihedral angle between the two benzene rings in 3 prevented the formation of the other D 2h , C 2v , and C s isomers under a high reaction temperature by keeping a good yield (48%). The methoxy groups in 5 were exchanged with hexyloxy groups by cleavage with BBr 3 and subsequent ether formation. We also tried to prepare 1 from 3-(2 ,6 -di(hexyloxy)phenyl)phthalonitrile; however, its yield was quite low (less than 1%) under the same reaction conditions as those used for 3. The large steric hindrance of hexyloxy groups would diminish the approach of using four phthalonitriles to form the Pc ring. The resulting Pc 1 can dissolve in many solvents except for alcohol and water, and it showed sharp, simple, and assignable 1 H-NMR spectra under a 1 × 10 −2 mol/dm 3 concentration at 25 • C ( Figure 2). The wide solubilities in the solvents and the sharp 1 H-NMR peaks at a high concentration indicate good dispersion as monomeric species without the formation of intermolecular aggregates in solvents, due to the steric hindrance of 2,6-dihexyloxybenzene substituents at the four α-positions of the Pc ring in 1.  Various asymmetric Pc rings (AAAB, ABAB, and AABB types) have been prepared through several approaches such as the statical mixing, the ring-expansion of subphthalocyanines, and the control of the steric repulsion of two different phthalonitriles [13]. The selective preparation of the ABAB-type Pcs has been shown to construct multicomponent molecular architectures, having linear arrangements. Torres et al. succeeded in the efficient synthesis of ABAB-type Pcs by using 3,6-di(3′,5′bis(trifluoromethyl)phenyl)phthalonitrile [14]. Since the attachment of two phenyl groups in the 3 and 6 positions of phthalonitriles is not enough to avoid self-condensation [15], the introduction of additional bulky substituents into the side benzenes is key to inhibiting the formation of distorted Pcs and AABB-type Pcs. We expect that the introduction of two methoxy groups at the 2 and 6 positions of the side benzenes will enhance the selectivity for the formation of the ABAB-type Pc. First, a Pc ring was not obtained by the tetramerization of 2 under the reported condensation conditions [15], revealing that the attachment of two 2,6-dihexyloxybenzene substituents at positions 3 and 6 of phthalonitrile interfered with the self-condensation of 2 into the distorted Pc ring. The   Various asymmetric Pc rings (AAAB, ABAB, and AABB types) have been prepared through several approaches such as the statical mixing, the ring-expansion of subphthalocyanines, and the control of the steric repulsion of two different phthalonitriles [13]. The selective preparation of the ABAB-type Pcs has been shown to construct multicomponent molecular architectures, having linear arrangements. Torres et al. succeeded in the efficient synthesis of ABAB-type Pcs by using 3,6-di(3′,5′bis(trifluoromethyl)phenyl)phthalonitrile [14]. Since the attachment of two phenyl groups in the 3 and 6 positions of phthalonitriles is not enough to avoid self-condensation [15], the introduction of additional bulky substituents into the side benzenes is key to inhibiting the formation of distorted Pcs and AABB-type Pcs. We expect that the introduction of two methoxy groups at the 2 and 6 positions of the side benzenes will enhance the selectivity for the formation of the ABAB-type Pc. First, a Pc ring was not obtained by the tetramerization of 2 under the reported condensation conditions [15], revealing that the attachment of two 2,6-dihexyloxybenzene substituents at positions 3 and 6 of phthalonitrile interfered with the self-condensation of 2 into the distorted Pc ring. The ABAB-type Pc 2 was synthesized as a structural isomer of 1 by mixing phthalonitrile and 4. The Various asymmetric Pc rings (AAAB, ABAB, and AABB types) have been prepared through several approaches such as the statical mixing, the ring-expansion of subphthalocyanines, and the control of the steric repulsion of two different phthalonitriles [13]. The selective preparation of the ABAB-type Pcs has been shown to construct multicomponent molecular architectures, having linear arrangements. Torres et al. succeeded in the efficient synthesis of ABAB-type Pcs by using 3,6-di(3 ,5 -bis(trifluoromethyl)phenyl)phthalonitrile [14]. Since the attachment of two phenyl groups in the 3 and 6 positions of phthalonitriles is not enough to avoid self-condensation [15], the introduction of additional bulky substituents into the side benzenes is key to inhibiting the formation of distorted Pcs and AABB-type Pcs. We expect that the introduction of two methoxy groups at the 2 and 6 positions of the side benzenes will enhance the selectivity for the formation of the ABAB-type Pc. First, a Pc ring was not obtained by the tetramerization of 2 under the reported condensation conditions [15], revealing that the attachment of two 2,6-dihexyloxybenzene substituents at positions 3 and 6 of phthalonitrile interfered with the self-condensation of 2 into the distorted Pc ring. The ABAB-type Pc 2 was synthesized as a structural isomer of 1 by mixing phthalonitrile and 4. The MALDI-TOF mass spectrum of the reaction mixture during the mixed condensation showed three mass peaks at m/z 526, 798, and 1070 g/mol, corresponding to Li 2 Pc, AAAB containing one isoindole (B) functionalized with two bulky bis(2,6-dimethoxy)phenyl units, and ABAB (or AABB) types. Compound 6 with m/z 1058 g/mol was successfully separated from the mixture by column chromatography and preparative HPLC. The 1 H-NMR spectrum of 2 exhibited only five peaks in the aromatic region, indicating the formation of an ABAB-type Pc (Figure 3) [7]. Furthermore, the proton signal for the two inside protons in the Pc ring was located at −0.51 ppm, suggesting no distortion of the Pc ring. Figure 4a,b show the absorption and fluorescence spectra of 1 and 2 in CH 2 Cl 2 . A comparison of the spectral shapes and peak positions for both spectra of 1 and 2 showed excellent agreement, revealing that the difference in molecular symmetries for 1 and 2 did not affect the electronic conditions of their Pc rings. Thus, structural isomers 1 and 2 with C 4h and D 2h molecular symmetries were successfully synthesized. Eight flexible hexyloxy chains in 1 and 2 were placed on both sides of the Pc plane and partially covered with a Pc skeleton ( Figure 5).
Molecules 2020, 25, x 4 of 11 MALDI-TOF mass spectrum of the reaction mixture during the mixed condensation showed three mass peaks at m/z 526, 798, and 1070 g/mol, corresponding to Li2Pc, AAAB containing one isoindole (B) functionalized with two bulky bis(2,6-dimethoxy)phenyl units, and ABAB (or AABB) types. Compound 6 with m/z 1058 g/mol was successfully separated from the mixture by column chromatography and preparative HPLC. The 1 H-NMR spectrum of 2 exhibited only five peaks in the aromatic region, indicating the formation of an ABAB-type Pc ( Figure 3) [7]. Furthermore, the proton signal for the two inside protons in the Pc ring was located at −0.51 ppm, suggesting no distortion of the Pc ring. Figure 4a,b show the absorption and fluorescence spectra of 1 and 2 in CH2Cl2. A comparison of the spectral shapes and peak positions for both spectra of 1 and 2 showed excellent agreement, revealing that the difference in molecular symmetries for 1 and 2 did not affect the electronic conditions of their Pc rings. Thus, structural isomers 1 and 2 with C4h and D2h molecular symmetries were successfully synthesized. Eight flexible hexyloxy chains in 1 and 2 were placed on both sides of the Pc plane and partially covered with a Pc skeleton ( Figure 5).   MALDI-TOF mass spectrum of the reaction mixture during the mixed condensation showed three mass peaks at m/z 526, 798, and 1070 g/mol, corresponding to Li2Pc, AAAB containing one isoindole (B) functionalized with two bulky bis(2,6-dimethoxy)phenyl units, and ABAB (or AABB) types. Compound 6 with m/z 1058 g/mol was successfully separated from the mixture by column chromatography and preparative HPLC. The 1 H-NMR spectrum of 2 exhibited only five peaks in the aromatic region, indicating the formation of an ABAB-type Pc ( Figure 3) [7]. Furthermore, the proton signal for the two inside protons in the Pc ring was located at −0.51 ppm, suggesting no distortion of the Pc ring. Figure 4a,b show the absorption and fluorescence spectra of 1 and 2 in CH2Cl2. A comparison of the spectral shapes and peak positions for both spectra of 1 and 2 showed excellent agreement, revealing that the difference in molecular symmetries for 1 and 2 did not affect the electronic conditions of their Pc rings. Thus, structural isomers 1 and 2 with C4h and D2h molecular symmetries were successfully synthesized. Eight flexible hexyloxy chains in 1 and 2 were placed on both sides of the Pc plane and partially covered with a Pc skeleton ( Figure 5).    Thermogravimetric analyses of 1 and 2 showed that the weight-losses started at around 300 °C under N2 atmosphere, indicating their thermal stability up to 300 °C (Figures S1 and S2). The thermal phase transition behaviors of 1 and 2 were checked by using a temperature-controlled polarizing optical microscope (TPOM) and differential scanning calorimetry (DSC) analysis. Compounds 1 and 2 melted at 120 and 130 °C, respectively, and the liquids showed no birefringence under POM observation. Liquid-crystalline Pcs with flexible alkyl chains at peripheral positions of the Pc core possessed two transitions, that is: a crystalline phase to a mesophase, and then a mesophase to an isotropic liquid [6]. At the first transition between the crystalline phase to the mesophase, the alkyl side chains in the liquid crystalline Pcs started to melt while maintaining the stack of the Pc molecules. The π-π stacking interaction in the Pc stacks could break at the second transition from the mesophase to the isotropic liquid. In contrast, the DSC profile of 1 displayed only one reversible transition at 121 and 70 °C upon heating and cooling runs at 10 °C/min ( Figure S3). This transition enthalpy (58.0 kJ/mol) roughly agreed with the reported melting enthalpy of side hexyl chains in 2,3,9,10,16,17,24octa(hexyloxy)phthalocyanine [16]. According to the results of TPOM and DSC for 1, the observed transition can be assigned to the melting point from crystal to isotropic liquid. Compound 1, possessing relatively short alkyl chains, exhibited a significantly lowed melting point compared with the reported values for Pcs with hexyl chains [17]. On cooling from the isotropic liquid, a birefringence texture appeared for the whole domain of 1 through crystallization (Figure 6a). An atomic force microscope (AFM) image of a thin film of 1 showed assemblies of short needles 30 nm in width (Figure 6b). Thermogravimetric analyses of 1 and 2 showed that the weight-losses started at around 300 • C under N 2 atmosphere, indicating their thermal stability up to 300 • C (Figures S1 and S2). The thermal phase transition behaviors of 1 and 2 were checked by using a temperature-controlled polarizing optical microscope (TPOM) and differential scanning calorimetry (DSC) analysis. Compounds 1 and 2 melted at 120 and 130 • C, respectively, and the liquids showed no birefringence under POM observation. Liquid-crystalline Pcs with flexible alkyl chains at peripheral positions of the Pc core possessed two transitions, that is: a crystalline phase to a mesophase, and then a mesophase to an isotropic liquid [6]. At the first transition between the crystalline phase to the mesophase, the alkyl side chains in the liquid crystalline Pcs started to melt while maintaining the stack of the Pc molecules. The π-π stacking interaction in the Pc stacks could break at the second transition from the mesophase to the isotropic liquid. In contrast, the DSC profile of 1 displayed only one reversible transition at 121 and 70 • C upon heating and cooling runs at 10 • C/min ( Figure S3). This transition enthalpy (58.0 kJ/mol) roughly agreed with the reported melting enthalpy of side hexyl chains in 2,3,9,10,16,17,24-octa(hexyloxy)phthalocyanine [16]. According to the results of TPOM and DSC for 1, the observed transition can be assigned to the melting point from crystal to isotropic liquid. Compound 1, possessing relatively short alkyl chains, exhibited a significantly lowed melting point compared with the reported values for Pcs with hexyl chains [17]. On cooling from the isotropic liquid, a birefringence texture appeared for the whole domain of 1 through crystallization (Figure 6a). An atomic force microscope (AFM) image of a thin film of 1 showed assemblies of short needles 30 nm in width (Figure 6b). The molecular arrangement of Pcs in the crystalline phase were analyzed on the basis of the temperature-controlled absorption spectra and X-ray diffraction patterns (XRD). The absorption spectral shape for the Q bands of Pcs is known to be sensitive to the local environment of individual molecules [16]. Figure 7a shows the absorption spectrum of the 1 film prepared by cooling from an isotropic liquid to room temperature. The Q band for the 1 film at room temperature was slightly broadened, and the Q band position was red-shifted from 705 nm in solution to 722 nm. The emission peak position was also shifted to a longer wavelength by 19 nm. The spectrum above the melting point was sharpened, and the maximum of the Q band peaks was shifted to a shorter wavelength. According to the molecular exciton theory [18], the red shift of the Q band suggests the parallel alignment of Pcs having inline transition dipoles. Whereas many planar Pcs show blue shift in the Q band to support the formation of columnar aggregates, through π-π interaction among Pcs, the bulky 2,6-dihexyloxybenzene substituents in 1 served to prevent the formation of stacks of Pc molecules. The structures of the crystalline phase and isotopic liquid of 1 were determined by XRD measurements at room temperature and at 140 °C (Figure 7b). The XRD pattern of 1 at 140 °C displayed only a broad and diffuse halo around 0.48 nm, which could be ascribed to the liquid-like disorder in alkyl chains. Upon cooling from 140 °C to room temperature, several broad reflections appeared at 2θ = 3-25 degree. The three reflections emerging at 1.2 nm, 0.6 nm, and 0.4 nm in a space ratio of 1:1/2:1/3 indicated that the crystalline 1 contained a lamellar structure. Judging from the simulated molecular dimensions of 1 by Gaussian 16 (Figure 4), the observed distance of 1.2 nm was shorter than the estimated molecular length of 1 with fully elongated hexyloxy chains, i.e., 1.7 nm. This implied that the lamellar layers may have originated from the head to tail interdigitated structure of the flexible hexyl chains on both sides of the Pc plain (Figure 7c). The other reflections at 1.5 and 2.1 nm coincided with the simulated side and diagonal lengths of the square α-substituted Pc plane, suggesting the formation of lateral assemblies of Pc rings in the lamellar structure (Figure 7d). However, the weak and broad XRD reflections for 1 suggest a short molecular ordering in the crystalline phase. The molecular arrangement of Pcs in the crystalline phase were analyzed on the basis of the temperature-controlled absorption spectra and X-ray diffraction patterns (XRD). The absorption spectral shape for the Q bands of Pcs is known to be sensitive to the local environment of individual molecules [16]. Figure 7a shows the absorption spectrum of the 1 film prepared by cooling from an isotropic liquid to room temperature. The Q band for the 1 film at room temperature was slightly broadened, and the Q band position was red-shifted from 705 nm in solution to 722 nm. The emission peak position was also shifted to a longer wavelength by 19 nm. The spectrum above the melting point was sharpened, and the maximum of the Q band peaks was shifted to a shorter wavelength. According to the molecular exciton theory [18], the red shift of the Q band suggests the parallel alignment of Pcs having inline transition dipoles. Whereas many planar Pcs show blue shift in the Q band to support the formation of columnar aggregates, through π-π interaction among Pcs, the bulky 2,6-dihexyloxybenzene substituents in 1 served to prevent the formation of stacks of Pc molecules. The structures of the crystalline phase and isotopic liquid of 1 were determined by XRD measurements at room temperature and at 140 • C (Figure 7b). The XRD pattern of 1 at 140 • C displayed only a broad and diffuse halo around 0.48 nm, which could be ascribed to the liquid-like disorder in alkyl chains. Upon cooling from 140 • C to room temperature, several broad reflections appeared at 2θ = 3-25 degree. The three reflections emerging at 1.2 nm, 0.6 nm, and 0.4 nm in a space ratio of 1:1/2:1/3 indicated that the crystalline 1 contained a lamellar structure. Judging from the simulated molecular dimensions of 1 by Gaussian 16 (Figure 4), the observed distance of 1.2 nm was shorter than the estimated molecular length of 1 with fully elongated hexyloxy chains, i.e., 1.7 nm. This implied that the lamellar layers may have originated from the head to tail interdigitated structure of the flexible hexyl chains on both sides of the Pc plain (Figure 7c). The other reflections at 1.5 and 2.1 nm coincided with the simulated side and diagonal lengths of the square α-substituted Pc plane, suggesting the formation of lateral assemblies of Pc rings in the lamellar structure (Figure 7d). However, the weak and broad XRD reflections for 1 suggest a short molecular ordering in the crystalline phase.  Figure 8a shows the DSC profiles of ABAB-type 2 upon heating and cooling runs at 2 °C/min. During the first heating runs from 30 to 200 °C, 2 exhibited one endothermic peak at 130 °C. Subsequent cooling at 2 °C/min showed an exothermic peak at 95 °C, and the transition enthalpies for the heating and cooling processes were comparable. When 2 was cooling from an isotropic liquid at 2 °C/min, birefringent short needles appeared at 95 °C under TPOM (Figure 8b), and sharp and intense peaks in the XRD measurement were detected (Figure 8c). According to an analysis of the XRD pattern, 2 crystal contained two crystal structures possessing different monoclinic lattices of Pcs. The XRD peaks, as indicated by * in Figure 8c, can be indexed according to a monoclinic lattice with Pcs with a unit cell with the parameters a = 2.31 nm, b = 2.06 nm, c = 0.41 nm, and α = 94° (Figure 8d). The center-center distance of 2 along the a-axis agreed with the simulated molecular length with elongated hexyl chains. The difference between the a-and b-axes suggested the tilting of the Pc cores within the stacks. The Pc cores were probably tilted with respect to the c-axis, and the tilted angle of the cores in the stacks could be calculated to be 34° [19]. Two sharp XRD peaks at d = 0.34 and 0.41 nm suggested a long-range ordered stacking of Pcs and benzene rings within the crystals. Furthermore, the appearance of several sharp reflections in the wide-angle region suggested a dense packing of the hydrocarbon chains in the crystals. The absorption spectrum of crystalline 2 was broadened, and the maximum of the Q band was blue-shifted to 687 nm, indicating the formation of a cofacial stack of Pc molecules (Figure 8e). Thus, the Pc rings in 2 could form long-range ordered stacks while avoiding the steric hindrance of 2,6-dihexyloxybenzene substituents attached to the 1, 4, 15 and 18 positions of the Pc rings due to slow cooling from an isotropic liquid (Figure 8f).  Figure 8a shows the DSC profiles of ABAB-type 2 upon heating and cooling runs at 2 • C/min. During the first heating runs from 30 to 200 • C, 2 exhibited one endothermic peak at 130 • C. Subsequent cooling at 2 • C/min showed an exothermic peak at 95 • C, and the transition enthalpies for the heating and cooling processes were comparable. When 2 was cooling from an isotropic liquid at 2 • C/min, birefringent short needles appeared at 95 • C under TPOM (Figure 8b), and sharp and intense peaks in the XRD measurement were detected (Figure 8c). According to an analysis of the XRD pattern, 2 crystal contained two crystal structures possessing different monoclinic lattices of Pcs. The XRD peaks, as indicated by * in Figure 8c, can be indexed according to a monoclinic lattice with Pcs with a unit cell with the parameters a = 2.31 nm, b = 2.06 nm, c = 0.41 nm, and α = 94 • (Figure 8d). The center-center distance of 2 along the a-axis agreed with the simulated molecular length with elongated hexyl chains. The difference between the a-and b-axes suggested the tilting of the Pc cores within the stacks. The Pc cores were probably tilted with respect to the c-axis, and the tilted angle of the cores in the stacks could be calculated to be 34 • [19]. Two sharp XRD peaks at d = 0.34 and 0.41 nm suggested a long-range ordered stacking of Pcs and benzene rings within the crystals. Furthermore, the appearance of several sharp reflections in the wide-angle region suggested a dense packing of the hydrocarbon chains in the crystals. The absorption spectrum of crystalline 2 was broadened, and the maximum of the Q band was blue-shifted to 687 nm, indicating the formation of a cofacial stack of Pc molecules (Figure 8e). Thus, the Pc rings in 2 could form long-range ordered stacks while avoiding the steric hindrance of 2,6-dihexyloxybenzene substituents attached to the 1, 4, 15 and 18 positions of the Pc rings due to slow cooling from an isotropic liquid (Figure 8f). In the DSC cooling run of 2 from an isotropic liquid at 20 °C/min, an exothermic peak was observed at 43 °C, which was lower than that obtained at 2 °C/min (Figure 9a). The XRD patterns for 2 exhibited only a broad halo (Figure 9b), and no birefringence was observed through TPOM. These results revealed that 2 was in a supercooled state due to rapid cooling from an isotropic liquid [20]. The second heating run from 10 °C revealed one exothermic crystallization peak at 43 °C and two endothermic peaks at 71 and 129 °C. The XRD patterns at 60 and 100 °C were comparable, and the intensities for the two peaks at 0.34 and 0.41 nm were weaker than those for the crystalline sample prepared by slower cooling at 2 °C/min (Figure 9b). Dark square domains including a latticed pattern were grown above 43 °C, supporting a square arrangement of Pcs in crystal (Figure 9c) [21]. The 2 film exhibited a red-shifted absorption band, observed at 726 nm (Figure 9d). Upon heating above the first endothermic peak, new shoulder peaks at 687 and 704 nm appeared, indicating a change in the Pc stacking mode. From these results, we assumed that the rapid temperature change could form metastable crystalline phases by diminishing the long-range ordered stacking of Pcs. In the DSC cooling run of 2 from an isotropic liquid at 20 • C/min, an exothermic peak was observed at 43 • C, which was lower than that obtained at 2 • C/min (Figure 9a). The XRD patterns for 2 exhibited only a broad halo (Figure 9b), and no birefringence was observed through TPOM. These results revealed that 2 was in a supercooled state due to rapid cooling from an isotropic liquid [20]. The second heating run from 10 • C revealed one exothermic crystallization peak at 43 • C and two endothermic peaks at 71 and 129 • C. The XRD patterns at 60 and 100 • C were comparable, and the intensities for the two peaks at 0.34 and 0.41 nm were weaker than those for the crystalline sample prepared by slower cooling at 2 • C/min (Figure 9b). Dark square domains including a latticed pattern were grown above 43 • C, supporting a square arrangement of Pcs in crystal (Figure 9c) [21]. The 2 film exhibited a red-shifted absorption band, observed at 726 nm (Figure 9d). Upon heating above the first endothermic peak, new shoulder peaks at 687 and 704 nm appeared, indicating a change in the Pc stacking mode. From these results, we assumed that the rapid temperature change could form metastable crystalline phases by diminishing the long-range ordered stacking of Pcs.

Conclusions
In summary, the crystalline structures of two structural isomers, 1 and 2, possessing different molecular symmetries, were investigated. The spatial overlapping of hexyloxy groups onto the πsurface of the Pc rings resulted in a significant decrease in the melting points, and large homogeneous domains were formed by cooling from the melting points. C4h isomer 1 organized into a layered structure by two-dimensional assembly without π-π stacking among Pcs. In contrast, D2h isomer 2 was able stack in the crystalline phase, and the ordering in the stacks depended on the cooling speeds from the isotropic liquid. Since Pc crystals have been used in several organic devices such as organic thin film transistors and organic photovoltaic cells due to their highly efficient electron or charge transportations [22,23], the thin films consisting of Pc crystals prepared by solution processes and thermal annealing have good potential as molecular components for such devices. Research on applying these Pcs to organic devices is in progress.

Conclusions
In summary, the crystalline structures of two structural isomers, 1 and 2, possessing different molecular symmetries, were investigated. The spatial overlapping of hexyloxy groups onto the π-surface of the Pc rings resulted in a significant decrease in the melting points, and large homogeneous domains were formed by cooling from the melting points. C 4h isomer 1 organized into a layered structure by two-dimensional assembly without π-π stacking among Pcs. In contrast, D 2h isomer 2 was able stack in the crystalline phase, and the ordering in the stacks depended on the cooling speeds from the isotropic liquid. Since Pc crystals have been used in several organic devices such as organic thin film transistors and organic photovoltaic cells due to their highly efficient electron or charge transportations [22,23], the thin films consisting of Pc crystals prepared by solution processes and thermal annealing have good potential as molecular components for such devices. Research on applying these Pcs to organic devices is in progress.

Conflicts of Interest:
The authors declare no conflict of interest.